Synthesis of imine bond containing insoluble polymeric ligand and its transition metal complexes, structural characterization and catalytic activity on esterification reaction

Abstract In this study, synthesis of insoluble polymeric ligand (L) and its transition metal complexes [Cu(L)Cl2]·2H2O (1), [Co(L)Cl2(H2O)2] (2) and [Ni(L)Cl2(H2O)2] (3), having the azomethine groups, were synthesized by the condensation reactions of the diamines and dialdehydes. The structural properties were characterized by the analytical and spectroscopic methods using by elemental analysis, Fourier Transform Infrared, Thermo Gravimetric Analysis, Powder X-ray Diffraction, magnetic susceptibility and Inductively Coupled Plasma. The solubilities of the synthesized polymeric materials were also investigated and found as insoluble some organic and inorganic solvents. Additionally, their catalytic performance was carried out for the esterification reaction of acetic acid and butyl acetate. The highest conversion rate is 75.75% by using catalyst 1. The esterification of butanol gave butyl acetate with 100% selectivity.


Introduction
Poly(azomethine)s, known as polyimines or Schiff base polymers [1] are obtained by derivating from different diamines and dialdehydes [2]. The presence of the nitrogen atom in their backbone makes them environmentally stable [3]. Polymers are described as high molecular weight molecules formed by the recurrence of monomeric units addicted with covalent bonds [4]. Among many ligands, polyazomethine polymers have attracted great interest due to their different properties such as conjugated backbone and good thermal stability [4], imine sites [5], ability to form metal chelates [6] and mechanical strength [7]. Transition metal complexes of polyazomethine polymers, prepared by the reaction of metal salts and polymers containing electron donor groups like -CH=N-, are showed high catalytic activities in various chemical reactions such as oxidation [8], epoxidation of olefins [9,10] and esterification reactions. However, heterogeneous catalysts indicate higher catalytic activity [11,12] and enantioselectivity [13] in comparison to homogeneous catalysts [14]. N-butyl acetate is an important compound in the chemical industry (Scheme 1). Primarily, it is used in paint, coating manufacture, and lacquer industry. Because of its lower impact on the environment, n-butyl acetate is able to replace the toxic and teratogenic effect of ethoxy ethyl acetate that is often used as a solvent [15,16].
In this study, we present synthesis and characterization of an insoluble polymeric ligand (L) and its metal com was heated under reflux for 1 h and then glutaraldehyde was added (4.005 g from water solution 25%, 10 mmol) in the reaction medium and it was boiled for three hours. All of the polymeric metal complexes were collected by filtration, washed with MeOH and dried under vacuum. The synthesized compounds were obtained as powder ( Figure 2) [17]. [Cu(L)

Esterification of butanol with acetic acid
The obtained butyl acetate was carried out at 25, 80 °C and boiling temperature in a three-necked flask (100 mL) equipped with a magnetic stirrer, a reflux condenser and a temperature controller in an oil bath. Butanol (4.95 g, 66.78 mmol) and acetic acid (4.083 g, 67.99 mmol) were added successively into the flask. After heating, the mixture is to be 25-80 °C-boiling temperature, the catalyst (0.05-0.10 g) was added to the mixture to initiate the reaction. The reaction mixture was stirred continuously for 4, 8 and 12 h. The products of the esterification reactions 4000-400 cm −1 ) FT-IR spectrometer. TGA was performed with a Perkin Elmer Pyris Diamond TG/DTA N 2 (50-800 °C range) at a heating rate of 10 °C/min. The characterization, selectivity % and catalytic conversion % studies of the esterification product, butyl acetate were analyzed by Thermo GC-FID. GC was performed using a Thermo GC-FID detector. A Perkin-Elmer Optima 2100 DV ICP-OES instrument was used for the ICP analysis. A Rigaku Miniflex system with CuKα radiation (λ = 1.54059 Å) was used for the PXRD studies. Magnetic susceptibility measurements were performed by using Sherwood Scientific magnetic susceptibility.

Synthesis of polymeric schiff base ligand
The polymeric Schiff base ligand were prepared by refluxing 2,4-diamino toluene (1.222 g, 10 mmol) with corresponding glutaraldehyde (4.005 g in water solution 25%, 10 mmol) in methanol (50 mL) for 3 h. The dark brown solution was filtered, and insoluble solid was washed 2 times with 20 mL methanol. It was dried under vacuum and reaction yield was determined as 92.6% (Figure 1

Results and discussion
The metal compounds were synthesized according to appropriate methods. For the characterization of obtained the polyimine ligand and its metal complexes were characterized by melting point, elemental analysis, TGA, FT-IR, ICP, XRD analysis, and magnetic susceptibility. The synthesized compounds were insoluble so they can be used as heterogenous catalysts. Resolution of catalyst 1 is shown in Table 1.

IR spectra
A strong and broad absorption band at the 1615 cm −1 shown by the synthesized polymeric ligand is attributable to the υ(C=N) stretching. In the complexes, this band shifted between 1616-1634 cm −1 indicating the coordination of azomethine nitrogen to the metal. This is supported by the appearance of new band in the region 584-699 cm −1 due to metal ligand bonding. The absorption bands relative to υ(O-H) stretching bands in the range of 3442-3213 cm −1 is shown the coordination of water to metal for the metal complexes [18]. The IR spectra are given in Table 2 and Figures S1-S4.

PXRD studies
Powder diffraction data 2θ values of the complexes are shown in Figure 3 and Table 3. The powder XRD analyses of the compounds have been performed in order to determine the information of non-polycrystalline material because it couldn't be obtained suitable crystals for single crystal X-ray analysis. Therefore the powder XRD    Table 3. The FWHM is the Bragg diffraction angle (b) and b is the full width at half maximum. The density (d) of the complex was determined by the floatation method in a saturated solution of KBr, NaCl and benzene separately. The all values agree well with the suggested structure of the complexes.
analysis of metal complexes was found to be amorphous in nature instead of crystalline. The indexing and calculations of unit cell parameters were performed using Powder-X software and scattering angles (2θ) corresponding to the each reflection, inter-planar spacing (d) along with Miller's indices and lattice constants were evaluated for complexes. The parameters like 2-Theta,

Molecular weight distribution of the polymers
It was performed solubility tests for synthesized polymers. As a result of the tests, we did not solved the structures in any organic and inorganic solvents (Table S1). So we could not performed GPC analysis to determination of the molecular weight of the polymers. After that, insoluble polymers were analysized with Quadrupole Timeof-flight Mass Spectrometry (Q-TOF MS) (maximum mass range: m/z: 17.000) and molecular weight of polymers could not be determined. This polymers have relatively high molecular weight, estimated to be in excess of 20.000 although the insolubility of the polymers have prevented exact determination [20].

Catalytic activity
Polymeric complexes have seldom been used as a heterogeneous catalyst for the esterification of butanol with acetic acid to butyl acetate [21]. There have been no reports on the esterification of butanol and acetic acid to butyl acetate using polyazomethine polymeric complexes, although butanol esterification reactions catalyzed by other types of the first row metal complexes in homogeneous and heterogeneous mediums [22]. In most of the cases, homogeneous acids and other metal complexes have been used for different catalytic conversion reactions. Homogeneous catalysis process has several disadvantages such as the product purification and reaction conditions. To avoid the loss of catalyst and for its recovery, many attempts have been taken, such as intercalating or

Magnetic susceptibility of the complexes
The magnetic susceptibilities of the polymeric transition metal complexes were determined using the Evans balance at room temperature in the solid state. The magnetic correction for each complexes was estimated using Pascal's constants. The magnetic moment data are shown in Table  2. According to the magnetic moment results, complex 1 has tetrahedral or square planar geometry;

Thermal analysis studies
Thermogravimetric analysis (TGA) was carried out to examine the thermal stabilities of the polymeric complexes.  To determine the catalytic conversion value without catalyst, one more control group experimental was performed. The esterification reaction was performed without catalyst and ~40% conversion value was observed as shown in the case of similar work [23]. Catalytic performance of the ligand was also done under same catalytic conditions. The GC/MS studies showed that 58% of conversion was observed using polymeric ligand as a catalyst. These studies supported that ligand is not showed high catalytic activity on esterification reaction as like synthesized heterogeneous catalysts.
After the catalytic studies, the catalysts filtered and washed with ether to avoid remained ester residues. Metal encapsulating the metal complex into the layered compounds or within the cavities of a porous solid (e.g., zeolites), binding the metal complex to a polymeric matrix and employing the steric hindrance. Percent selectivity and characterization studies of the butyl acetate were carried out by using GC-FID. The esterification of butanol gave butyl acetate with 100% selectivity. The catalytic activity of the synthesized polymeric complexes was evaluated for the esterification of butanol in the presence of dichloromethane using a standard GC analysis technique. Table  4 summarizes the results, percentage of butanol conversion in the different reaction conditions. Conversion values were determined for butanol and butyl acetate calibration curves. To determine the performance of the catalyst, the yield butyl acetate formation from butanol and acetic acid was plotted as a function of different reaction conditions such as temperature, catalyst amount and reaction time.
Although it was obtained low product conversion at room catalysts can be readily recycled more than three times (Table S2). One of the best advantages of the insoluble polymeric structure as a catalyst could be accepted porosity of the surface of the catalysts. Insoluble low molecular weight catalyst has no 3D structure at the reaction condition therefore the expectation of that the rate of the reaction will be lower than the catalysts having 3D surface morphology. Another point we can concluded from our previous studies and TGA results, the polymeric insoluble catalysts is longer lifetime than the insoluble low molecular weight catalysts. Additionally, it is anticipated that durability of the 3D structure is much better than the monomers during the different reaction conditions.

Conclusions
We . The synthesized polymeric compounds were characterized by using analytical and spectroscopic methods. The polymeric copper complex has higher catalytic activity than the Co(II) and Ni(II) transition metal complexes containing polyimine or polymeric Schiff base ligand as a heterogeneous catalyst. Because of the presence of the imine bridges, all the complexes are insoluble in hot/cold many common organic and inorganic solvents (Table S1). The solubility feature is important for the heterogeneous catalysts. Butyl acetate can be easily obtained by catalytic esterification of precursor by using butanol, acetic acid and catalysts. The esterification of butanol and acetic acid with 75.75% conversion gave butyl acetate with 100% selectivity. To the best of our knowledge, this is the first recorded on the esterification of butanol and acetic acid to butyl acetate by using complex 1 as a catalyst. In addition, catalytic conversions are increasing with increasing temperature but do not increase catalytic conversions with the amount of increased catalyst.

Disclosure statement
No potential conflict of interest was reported by the authors.

İlyas Gönül
http://orcid.org/0000-0001-7747-9441 complexes were dried and TG analysis were performed secondly. After the TG analysis, no difference was observed in the thermal curves of the catalysts (Figures S8-S10). Although the loss of H 2 O was observed at 70-100 °C, it was observed that there was no change in the structure of the polymer in catalytic studies at boiling temperature. Since catalytic studies were carried out in solution medium, it is possible that water molecules separated at the end of the experiment were re-bound to the structure. The obtained results supported that there is no change in the lattice structure of water molecule in the polymeric structures.

Reaction mechanism for esterification of butyl acetate
The proposed mechanism of the esterification reaction is summarized in Figure 4. For easy description, the reproducible part of the synthesized polymer is abbreviated as R and R′ (i). When the catalytic activity of the ligand was examined, 58% conversion was obtained. The maximum yield of metal complexes was determined to be 75.75%. This result supported that the metal ion plays an active role in catalytic reaction, thus initiating the reaction with a proton separation by binding to the acetate ion (ii). Acetate ion attached to the complex structure is attached to the carbonyl carbon, and alcohol is bonded to the oxygen group, leaving the proton in the alcohol (iii). When the OH group in the final structure is separated by proton capture as H 2 O, ester formation is completed (iv). As the mechanism proceeds through the attachment of acetate ion to the metal, etheric structures is not form as by-products. This result was supported by GC-FID results. The polymeric catalysts synthesized for this reason were 100% selective in the esterification reaction. It is also believed that the chain structure of the polymeric catalyst helps the hydrophobic group of alcohol to approach the metal in position.

Separation and stability of catalyst
The major advantage of the use of heterogeneous catalysts is to recover the catalyst from the reaction mixture by simple filtration and recycle. The recovered heterogeneous catalysts can be reused in subsequent reactions. In order to assess the stability of the catalyst, the solid was filtrated at the end of the each reaction and washed with dichloromethane then dried at 50 °C. The dried catalyst was used under the same reaction conditions (butanol/acetic acid, 0.1 g polymeric catalysts, boiling temperature and 12 h). At the end of third reaction, butanol/acetic acid conversion did not change significantly. The recycling property is a very important parameter for a heterogeneous catalyst. This study showed that polymeric transition metal